Elastic and plastic deformations of charge density waves 486 carried on under electric fields on...
Embed Size (px)
Transcript of Elastic and plastic deformations of charge density waves 486 carried on under electric fields on...
HAL Id: jpa-00210720 https://hal.archives-ouvertes.fr/jpa-00210720
Submitted on 1 Jan 1988
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci- entific research documents, whether they are pub- lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Elastic and plastic deformations of charge density waves Denis Feinberg, J. Friedel
To cite this version: Denis Feinberg, J. Friedel. Elastic and plastic deformations of charge density waves. Journal de Physique, 1988, 49 (3), pp.485-496. �10.1051/jphys:01988004903048500�. �jpa-00210720�
Elastic and plastic deformations of charge density waves
D. Feinberg (*) and J. Friedel (**)
(*) Centre National de la Recherche Scientifique, Laboratoire d’Etudes des Propriétés Electroniques des Solides, associated with Université Scientifique, Technologique et Médicale de Grenoble, B.P. 166, 38042 Grenoble Cedex, France (**) Laboratoire de Physique des Solides, associé au CNRS, Université Paris-Sud, Centre d’Orsay, Bât. 510, 91405 Orsay Cedex, France
(Reçu le 23 septembre 1987, accept6 le 17 novembre 1987)
Résumé. 2014 Nous présentons une théorie élastique des déformations d’une O.D.C. sous l’effet d’un champ électrique, à l’aide d’un simple hamiltonien de phase. L’accent est mis sur la rigidité interne de la modulation qui ressemble en réalité à un « solide électronique », et sur l’anisotropic de ses constantes élastiques. Les déformations continues de l’O.D.C. sont décrites par un tenseur des déformations donné par les variations relatives du vecteur d’onde de la modulation. Les contraintes sont dues aux effets combinés du champ électrique externe et des points d’ancrage. Sous faible contrainte le condensat, globalement accroché, conserve la continuité de phase : la structure n’a pas de défauts. Sous de plus fortes contraintes des dislocations sont nucléées, mettant en jeu une variation locale d’amplitude de l’O.D.C. Nous décrivons le processus de nucléation pour des boucles élémentaires sous champ externe et comparons en conséquence les seuils pour le désancrage de l’O.D.C. des impuretés et des bords (surfaces et interfaces). Une longueur caractéristique est obtenue en dessous de laquelle l’ancrage aux contacts domine et une déformation cohérente (polarisation) apparaît.
Abstract. 2014 An elastic theory of CDW deformations under electric fields is presented, on the basis of a simple phase Hamiltonian. The emphasis is put on the internal rigidity of the modulation which indeed resembles an « electronic solid », and on the anisotropy of its elastic constants. CDW’s continous deformations are described by a strain tensor given by the relative variations of the wavevector of the modulation. Stresses occur due to the combined effect of external electric field and pinning points. Under low stresses the globally pinned condensate retains phase continuity : the structure has no defects. Under larger stresses dislocation loops are nucleated involving local amplitude variations of the CDW. We describe the nucleation process for elementary loops under an external field and compare as a consequence thresholds for impurity depinning and boundary depinning (surfaces or interfaces). A characteristic sample length is found under which contact pinning prevails and a coherent deformation (polarization) is built.
J. Phys. France 49 (1988) 485-496 MARS 1988,
Physics Abstracts 61.70 - 62.20 - 71.45
Since the first discovery of collective electronic conduction by sliding charge density waves (CDW) in 1976 , an important sum of work has been devoted to the understanding of these very unusual properties . Different classes of compounds, all quasi-unidimensional, share at this time the property of sliding CDW’s : tri and tetrachalcogenides as NbSe3, TaS3, (TaSe4)21 and (NbSe4)10/31, molyb- denum bronzes Ao.3MOO3 (A = K, Rb, Tl) and more recently TTF-TCNQ [2, 3]. Of all these compounds only NbSe3 remains metallic at low
temperature, the others becoming semiconductors with a Peierls gap opening on the nearly perfectly nested Fermi surface. The clearest evidence for sliding of the CDW -
the so-called Frohlich mode - comes from the observation of periodic « noise » generated by the motion over the underlying periodic pinning poten- tial [1, 2]. Pinning of the condensate by random impurities is most probably the cause of the finite threshold field for CDW motion and of the strong metastability effects [4, 5]. Deformations of the CDW have been proven to exist, especially under electric fields [6-9]. Furthermore NMR experiments
Article published online by EDP Sciences and available at http://dx.doi.org/10.1051/jphys:01988004903048500
carried on under electric fields on NbSe3  and Rbo,3Mo03  seem to give clear evidence of a coherent motion of the whole condensate. Unfortu-
nately, even if the basic physics are understood and reasonable theoretical models exist (Ref. [2a] Vol. I), up to now no synthetic picture is able.,to account for the rich and complex experimental situation. The quantum origin of CDW formation is well
understood : the Peierls instability  of the quasi one-dimensional Fermi surface at q = 2 kF induces the condensation of electron-hole pairs at q and - q, resulting in a modulation in real space of both the atomic positions and the electronic density, while a gap 2 4 opens at the Fermi level EF. The
question of deciding whether CDW motion results of macroscopic tunnelling of the condensate through impurities  or from a purely classical process [14, 15] is still controversial. In the first eventuality, apparently confirmed by interference experiments , these systems would be amongst the few known examples of macroscopic quantum phenomena. On the other hand, it is difficult to ascribe all the observed phenomena to such an effect. On the contrary, low time scale metastability properties are clearly the sign of large length scale relaxation, hardily described but by deformations of a classical medium. We shall restrict ourselves to such a classical approach and do not attempt to cover the eventual crossover to quantum effects. The lattice modulation and ensuing CDW can be
considered as a purely sinusoidal wave in a con- tinuum. In this approximation the electric charge density along the chains is
The CDW is locally described by its amplitude or by the gap 4, and by its phase cp respective to the fixed lattice. It can be alternatively characterized by a complex two-component order parameter I/J = (4/do ) e’o where do is the T = 0 gap for an undistorted CDW. As a consequence, such a system has to be compared to other systems described by two-component order parameters such as superfluids and superconductors, x-y magnets or some liquid crystals. The Bose condensation of electron-hole pairs at
± q , q = 2 kF [17, 18] gives rise to a coherence length
§, indeed very similar to the BCS coherence length and measuring the order of magnitude of the size of the electron-hole pair. In the chain direction it is given by Çll ’" IlvF/ 7r A where V F is the Fermi velocity. It can be much smaller in the transverse direction, being due to the weak interchain couplings. kF 1 being of the same order of magnitude as the parallel unit length a, , one sees that §jj lail - £F/11 which is of the order of several tenth, giving §jj -- 100 A as an order of magnitude. This shows that CDW electrons keep their itinerant character and are not truly localized by their effective interac- tion. An alternative model due to Aubry  considers the opposite case of a « polaronic crystal » valid in strong enough coupling. An heuristic argu- ment can be given to explain how real space electronic ordering can originate from a conden- sation of « large » electron-hole pairs in weak coupl- ing. One must take into account the fact that the effective mass for Frohlich electrons coupled to heavy ions is the Frohlich mass M ’" 102 to 103 me, thus the zero-point kinetic energy of the modulation is of order k 2/2 M, smaller than the interaction 4 which stabilizes the modulation. Thus the first of the two inequalities
expresses the conditions for a quantum « electron solid » to form, while the second one expresses that amplitude variations of the CDW can occur only on distances longer than the coherence length §. We want to point out that the rigidity of CDW’s,
as stressed by Anderson [4, 20] is an essential feature which has not received enough attention up to now. As a consequence one can hope to build an elastic description of CDW deformation and motion, similar to that of a three-dimensional solid. A few conditions must be put forward to justify such a picture. First, it is valid only at low temperature, far enough from the Peierls transition. The CDW actually softens close to
Tp due to the decrease of A and the first inequality of (1.4) might not be fulfilled anymore. Secondly, the following description assumes that all long-range Coulomb interactions internal to the CDW deg